W H I T E P A P E R
Six Parameters of Cost-Effective Metal Casting Design
Six Parameters of Cost-Effective Metal Casting DesignMetalcasting is simultaneously a simple process and a complicated one. From a very elementary view, metalcastersjust fill a mold with molten metal and let it solidify, forming a cast component. However, each of the different met-alcasting processes offer distinct advantages and benefits when matched with the proper alloy. Capitalizing on theseadvantages takes an understanding of the power of casting geometry and the marriage of casting process and alloy.
Designers may choose from a large number of metalcasting processes and materials to achieve the right combination for optimized success. These include green sand metalcasting, one of the most common processes,or metal molding methods, such as permanent mold, diecasting and centrifugal casting. Other techniques useceramic slurries for molding, such as investment (lost wax) and plaster casting, or patterns made of styrofoam orno pattern at all as with rapid prototyping. Each of these processes offer unique benefits that may enhance a castcomponents design, surface finish, mechanical properties and/or dimensional tolerances. In addition, the processmay allow for a reduction in machining, coating or assembly costs.
The challenge for component designers is understanding the best combination of processes and technologies forcost-effective design. Due to the extensive geometric freedom offered by the metalcasting process, designers areprovided a blank palette to detail their engineered solutions.The geometric freedom of the metalcasting processallows multiple parts assembled together to become a single cast component, enhancing the finished componentsmaterial and mechanical properties and ultimately the end products effectiveness and productivity.
Six Steps to Success
The key to success lies in a better understanding ofthe relationship among geometry, various castingalloys and structure. There are six parameters(based on physics) that underlie cost-effective castingdesign as shown in Fig. 1.
All six, applied as a system, drive the geometry ofcasting design. Geometry is not only the result of casting design but is also the most powerfulweapon in creating successful casting design. Thissix-faceted system is capable of optimizing geometryfor castability, structure, downstream processing(machining and assembly) and process geometry(risering, gating, venting and heat transfer patterns)in the mold. The process geometry forms the castinggeometry.
Following these rules also eliminates the confusion that often results from following some of the rules of thumbthat have been developed over the years for common design situations. Further, the rules help when a design engi-neer leaves a familiar casting design realm for an unfamiliar one. For example, good aluminum bronze geometryis different than typical ductile iron geometry, and the molding process may need to supplement the different geometry with heat transfer techniques.
Quickly sorting through possible casting and process geometries by marking up blueprints or by making engineeringsketches is the way to find optimal system geometry. An elegant result of good sketched brainstorming can be asolid model of the casting and its process geometry, the basis of rapid prototyping and/or computerized testing.
Applying the System
Optimizing casting geometry using the six-parameter system is not difficult.The six casting and structural charac-teristics influence important variables in designing, producing and using metal castings.These variables include:
Casting method Surface integrity Design of casting sections Internal integrity Design of junctions Dimensional capability
between casting sections Cosmetic appearance
Casting Properties1. Fluid Life2. Solidification Shrinkage
a.Type (eutectic, directional and equiaxed)b.Volume (small, medium, large)
3. Slag/Dross Formation Tendency4. Pouring Temperature
Structural Properties5. Section Modulus (stiffness of casting geometry)6. Modulus of Elasticity (stiffness of alloy itself)
Fig. 1. Six parameters that drive cost-effective casting design
Casting geometry is the most powerful tool available to improve castability of the alloy and mechanical stiffness of the casting. Carefully planned geometry can offset alloy problems in fluid life, solidification shrinkage, pouringtemperature and slag/dross forming tendency. Section modulus, an attribute of structural geometry, has the capability to increase stiffness and/or reduce stress a capability that can be very important when applied to alloys with lower strength and stiffness. Modulus of elasticity, an alloys inherent stiffness, can be combined withsection modulus and section length to limit or allow deflection in a casting design.
To preview geometrys ability to influence the four characteristics of castability, consider the simple steel fabri-cation in Fig. 2a that was converted into carbon steel and gray iron casting designs, Figs. 2b and 2c, respectively. Thefabrication is a guide block to constrain low velocity/low load sliding motion, and it was welded from rectangularbar stock, subsequently milled, drilled and tapped. The geometries in 2b and 2c are considerably different as a consequence of differences among fluid life, solidification shrinkage type and amount, pouring temperature and tendency to form nonmetallic inclusions (See Junctions, Fig. 3).
Fig. 2. Shown here is the original steel fabrication (2a), a carbon steel casting design featuring propergeometry that suits its four casting characteristics (2b), and a gray iron casting featuring an entirely different geometry that is still based on its four casting alloy characteristics (2c).
Examining in more detail each of the six parameters that underlie cost-effective casting design illustrates their influence. The first four factors affect casting properties while the last two affect structural properties. Additionaldetails on each of these parameters can be found in Cost-Effective Casting Design, in the 2006 AFS CastingSource Directory.
1. Fluid Life
Fluid life more accurately defines the alloys liquid characteristics than does the traditional term fluidity. Moltenmetals fluidity is a dynamic property, changing as the alloy is delivered from a pouring ladle, die casting chamber,etc. into a gating system and finally into the mold or die cavity.
Fluid life affects the design characteristics of a casting, such as the minimum section thickness that can be cast reliably, the maximum length of a thin section, the fineness of cosmetic detail (like lettering and logos) and the accuracy with which the alloy fills the mold extremities.
2. Solidification Shrinkage
There are three distinct stages of shrinkage as molten metals solidify: liquid shrinkage, liquid-to-solid shrinkage andpatternmakers contraction.
Liquid shrinkage is the contraction of the liquid before solidification begins. It is not an important design consideration.
Liquid-to-solid shrinkage is the shrinkage of the metal mass as it transforms from the liquids disconnectedatoms and molecules into the structured building blocks of solid metal. The amount of solidification shrinkagevaries greatly from alloy to alloy.Table 1 provides a guide to the liquid-to-solid shrinkage of common alloys. Asshown, shrinkage can vary from low to high shrinkage volumes.
Alloys are further classifiedbased on their solidificationtype: directional, eutectic-typeand equiaxed (see definitions inTable 1). The type of solidifica-tion shrinkage in a casting is justas important as the amount ofshrinkage. Specific types ofgeometry can be chosen to con-trol internal integrity whensolidification amount or typesare a problem.
Patternmakers Contractionis the contraction that occursafter the metal has completelysolidified and is cooling to ambient temperature. This contraction changes the dimen-sions of the casting from thoseof liquid in the mold to thosedictated by the alloys rate ofcontraction. So, as the solidcasting shrinks away from themold walls, it assumes finaldimensions that must be pre-dicted by the pattern- or die-maker. Tooling design and con-struction must compensate forit. The unpredictable nature ofpatternmakers contraction makestooling adjustments inevitable.
3. Slag/Dross Formation
Among metalcasters, the termsslag and dross have slightly dif-ferent meanings. Slag typicallyrefers to high-temperature flux-ing of refractory linings of fur-naces/ladles and oxidation prod-ucts from alloying. Dross typically refers to oxidation or reoxidation products in liquid metal from reaction withair during melting or pouring, and can be associated with either high or low pouring temperature alloys.
Some molten metal alloys generate more slag/dross than others and are more prone to contain small, round-shaped nonmetallic inclusions trapped in the casting. Unless a specific application is exceedingly critical, a few smallrounded inclusions will not affect casting structure significantly. In most commercial applications, nonmetallic inclu-sions are only a problem if they are encountered during machining or appear in a functional as-cast cosmetic surface.
4. Pouring Temperature
The refractory characteristics and limitations of mold materials will affect the choice of the molding process anddesign. When pouring temperature approaches a mold material refractory limit, the heat transfer patterns of thecasting geometry become important.
Sand and ceramic materials with refractory limits of 3000-3300F (1650-1820C) are the most common mold materials. Metal molds, such as those used in diecasting and permanent molding, have temperature limitations.